Presentation on theme: "Applied CFD in the Metallurgical Industry"— Presentation transcript:
1Applied CFD in the Metallurgical Industry Jonas Alexis MEFOS AB
2Outline Why are MEFOS modelling Metallurgical processes What is applied CFD at MEFOSExample: Sulphur Refining of SteelTransport descriptionReaction modelReaction ZoneScalar equation modelEmpirical modelValidationTransport EquationSulphur refiningConclusions
3Why are MEFOS modelling metallurgical processes? The goal for the metallurgical industry is to achieve the material properties needed for production of a given product. This requires control of the amount of:Alloying elements (C, Si, Mn, Cr, Al ..)Other elements (S, N, H, P, Cu, Zn ..)Unwanted non-metallic particles (Inclusions). Also composition and size distributionContinuous measurement and sampling for process control is difficult in most process steps. The models are therefore needed for:Optimisation of the different process stepsDevelopment of process control systemsEnhanced understandingEducation
4What is applied CFD at MEFOS When fundamental models are missing or impossible to realize because of the lack of data, which is often the case, other methods need to be utilised.One example: Fundamental data needed to describe the slag/metal-interface in a stirred ladle during sulphur refining is missing. Instead, empirical models of that interface, based on sampling at the steel plant can be used. The use is necessary if sulphur-refining in a production ladle is to be simulated.
8Sulphur Refining Reaction Model Equation 1. Al is related to Al2O3Equation 2. Fe is related to FeOEquation 3. Mn is related to MnOEquation 4. Si is related to SiO2Equation 5. [S] is related to (S)O is related to:wt%O] = [wt%O]Al O + [wt%O]FeO +[wt%O]MnO + [wt%O]SiO +[wt%O]S232
9Reaction Zone Scalar Equation model Top part of a Plane in the in the ladle, through the open eyesReaction Zone (Mixed Steel and Slag)Slag PhaseGas flow Directed UpwardsSteel Phase
10Reaction Zone Sampling (Empirical model) Sampling in the ladleSamplerAfter sampling
11Reaction Zone Sampling (Empirical model) After sampling and quenching, each sample was mechanically opened. The metal bulk, slag bulk and slag-metal interface can be easily identified. Thereafter, the slag part was physically divided into a number of zones on the basis of the distance from the slag-metal interface. The width of each zone was not constant for all the samples. Small pieces of collected slag were analyzed using light optical microscope (LOM) and scanning electron microscope (SEM). The chemical compositions of the slag samples were analyzed and the sulphur contents were determined.
12Reaction Zone Empirical Model The figures shows schematically the contact of metal with the lowest layer of slag droplets and the flow of metal associated with slag droplets. The following assumptions are made:1. After stabilization of the flow, the whole slag layer is in droplet form.2. All slag droplets are spherical and having the same size and shape.3. The linear velocity of the metal along the periphery of the slag droplet is equal to the velocity of the bulk flow of the metal at the slag-metal interface.4. The contribution of the metal film covering each slag droplet to the rate of mass exchange is negligible.
13Reaction Zone Empirical Model The metal volume associated with each slag droplet can be expressed by:(1)The mass of the metal associated with all slag droplets is given by:(2)The average time to travel a distance of 2 r can be evaluated by(3)The time required to flush out all the metal can be written as(4)The flush-out rate of the metal in a unit cell can be expressed by:(5)Eqs. (2) to (5) lead to(6)
14Sulphur Refining and Reoxidation Model 0.0000.0020.0040.0070.0090.0110.0130.0150.0180.0200.0220.0240.0270.0290.0310.0300.0330.0360.0390.0410.0440.0470.0500.0530.0560.0590.0610.0640.0670.0701.1E-41.4E-41.6E-41.8E-42.2E-42.5E-42.7E-43.0E-43.3E-43.5E-43.8E-44.1E-44.4E-44.6E-44.9E-4[%S] [%Al] [%O][%S] [%Al] [%O]Steel/slag interface
15Validation Transport description Velocity measurements with graphite rods
16Validation Wave Height Model Simulated waveheightHeight aboveFluid Surface
17Validation Validation of Wave Height Model Bernoulli’s equation for incompressible flowComparison between Bernoulli and simulation
18Validation Transport Description Measuring positions in the ladleInduction stirrer12312Porous plugs for gas injection
19Validation Transport Description Velocity measurements with graphite rods
20Validation Transport Description Steel velocities in ladle during induction stirringPredicted
21Validation Sulphur Refining and Reoxidation For a validation of the ”Sulphur refining and reoxidation predictions from the model a comparison between predicted results and data from the industry was performed. Slag and Steel was sampled before and after the sulphur refining process. The process took 850 seconds and was performed in vacuum making it impossible to sample during the process. The two sets of Slag and Steel samples were analysed and used as input data and resulting Steel analysis respectively.
22Validation Sulphur Refining and Reoxidation Slag analysis Steel analysisMeaured Predicted
23ConclusionsFor a Qualitative description (Parametric studies) a simpler reaction zone model can be used.For a Quantitative description of Sulphur refining, the development of empirical models describing the reaction zone in a steel ladle must be utilised due to the lack of data prohibiting development of a fundamental model.